A 3D porous supramolecular architecture via π‒π assembly of 2D metal‒organic frameworks (MOFs): structure-versus-luminescence reversibility and gas adsorption properties
Wang, Chih-Chieh; Sheu, Gia-Bin; Ke, Szu-Yu; Shin, Chi-Yang; Cheng, Yu-Jen; Chen, Yi-Ting; Cho, Chia-Hsing; Ho, Mei-Lin; Chen, Wen-Tin; Liao, Ru-Hsio; Lee, Gene-Hsiang; Sheu, Hwo-Shuenn; CrystEngComm 17 (2015) 1264–; doi:10.1039/C4CE01849D

data_7218856
_publ_section_title
;
 A 3D porous supramolecular architecture via \p--\p assembly of 2D
 metal--organic frameworks (MOFs): structure-versus-luminescence
 reversibility and gas adsorption properties
;
_journal_issue                   6
_journal_name_full               CrystEngComm
_journal_page_first              1264
_journal_paper_doi               10.1039/C4CE01849D
_journal_volume                  17
_journal_year                    2015
_chemical_formula_sum            'C18 H14.2 N2 O5.1 S2 Zn'
_chemical_formula_weight         469.60
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2014-10-29 deposited with the CCDC.
2014-11-20 downloaded from the CCDC.
;
_cell_angle_alpha                67.610(1)
_cell_angle_beta                 80.961(1)
_cell_angle_gamma                68.932(1)
_cell_formula_units_Z            2
_cell_length_a                   9.5666(4)
_cell_length_b                   11.5400(5)
_cell_length_c                   11.8627(5)
_cell_measurement_temperature    295(2)
_cell_volume                     1129.64(8)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.984
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0213
_diffrn_reflns_av_sigmaI/netI    0.0283
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            12869
_diffrn_reflns_theta_full        27.50
_diffrn_reflns_theta_max         27.50
_diffrn_reflns_theta_min         1.86
_exptl_absorpt_coefficient_mu    1.300
_exptl_absorpt_correction_T_max  0.9324
_exptl_absorpt_correction_T_min  0.8170
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2001)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.381
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             478
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.123
_refine_diff_density_min         -0.402
_refine_diff_density_rms         0.119
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.088
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     255
_refine_ls_number_reflns         5106
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.106
_refine_ls_R_factor_all          0.0491
_refine_ls_R_factor_gt           0.0463
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1181P)^2^+0.2341P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1579
_refine_ls_wR_factor_ref         0.1604
_reflns_number_gt                4655
_reflns_number_total             5106
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4ce01849d2.cif
_cod_data_source_block           ic13509_ht_to_rt-1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 7218854--7218856.cif.
;
_cod_original_sg_symbol_H-M      P-1
_cod_original_formula_sum        'C18 H14.20 N2 O5.10 S2 Zn'
_cod_database_code               7218856